On Verdigris, Part I: Synthesis, Crystal Structure Solution and Characterization of the 1-2-0 phase (Cu3(CH3COO)2(OH)4)
Bette, Sebastian; Kremer, Reinhard; Eggert, Gerhard; Tang, Chiu; Dinnebier, Robert E.; Dalton Trans.  (2017) –; doi:10.1039/C7DT03288A

data_7044485
_publ_section_title
;
 On Verdigris, Part I: Synthesis, Crystal Structure Solution and
 Characterization of the 1-2-0 phase (Cu3(CH3COO)2(OH)4)
;
_journal_name_full               'Dalton Trans.'
_journal_paper_doi               10.1039/C7DT03288A
_journal_year                    2017
_chemical_formula_moiety         '2(C2 H3 O2), 4(O H), (Cu)'
_chemical_formula_sum            'C4 H10 Cu3 O8'
_chemical_formula_weight         376.75
_chemical_melting_point          'decomposition above 160\%C'
_chemical_name_common            'Cu(CH3-COO)2*2Cu'(OH)2*0H2O, 1-2-0 phase'
_chemical_properties_physical    Heat-sensitive
_space_group_IT_number           61
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_audit_creation_method           TOPAS
_audit_update_record
;
2017-07-31 deposited with the CCDC.
2017-10-10 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   20.97417(14)
_cell_length_b                   7.20756(3)
_cell_length_c                   13.12202(6)
_cell_measurement_temperature    303
_cell_volume                     1983.690(18)
_diffrn_ambient_temperature      303
_diffrn_detector
; 
 multi MYTHEN II (Dectris)   
;
_diffrn_measurement_device_type  'synchrotron radiation'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.8260
_diffrn_source_type              'synchrotron radiation'
_exptl_absorpt_process_details
;   
 ?
;
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    2.52
_exptl_crystal_description       'microcrystalline powder'
_exptl_crystal_preparation       'Magnetic properties'
_pd_calc_method                  'Rietveld Refinement'
_pd_instr_location
; 
'SLS (Swiss Light Source)'
;
_pd_meas_2theta_range_inc        0.001
_pd_meas_2theta_range_max        60.0
_pd_meas_2theta_range_min        3.0
_pd_meas_scan_method             step
_pd_proc_2theta_range_inc        0.001
_pd_proc_2theta_range_max        60.0
_pd_proc_2theta_range_min        3.0
_pd_proc_info_data_reduction     binning
_pd_proc_info_excluded_regions
;
 ?
;
_pd_proc_ls_background_function
;   
'Chebyshev polynomial'
;
_pd_proc_ls_peak_cutoff          0.00100
_pd_proc_ls_profile_function
;
 Fundamental parameters
;
_pd_proc_ls_prof_R_factor        0.0868
_pd_proc_ls_prof_wR_expected     0.0111
_pd_proc_ls_prof_wR_factor       0.0832
_pd_spec_mounting
; 
'0.5 mm glass capillary'
;
_pd_spec_mount_mode              transmission
_pd_spec_shape                   cylinder
_refine_ls_number_parameters     78
_refine_ls_R_Fsqd_factor         0.0412
_cod_data_source_file            c7dt03288a2.cif
_cod_data_source_block           Cu3(CH3COO)2(OH)4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_original_cell_volume        1983.691(18)
_cod_original_sg_symbol_H-M      Pbca
_cod_database_code               7044485